You inspire … we materialize®
The World’s Leading Manufacturer of Plastic Stock Shapes
Plastics increasingly replace traditional materials such as bronze, stainless
steel, cast iron and ceramics. They are chosen for improved performance and TABLE OF CONTENTS
cost reduction. Plastics can: Coolants. . . . . . . . . . . . . . . . . . . . . . 5
• Reduce Weight
• Eliminate Corrosion Annealing . . . . . . . . . . . . . . . . . . . . . 6
• Improve Wear Performance in Unlubricated Conditions Machinability. . . . . . . . . . . . . . . . . . . 9
• Reduce Noise Drilling . . . . . . . . . . . . . . . . . . . . . . . 10
• Increase Part Life
• Insulate, both Thermally and Electrically Sawing . . . . . . . . . . . . . . . . . . . . . . . 16
Typical applications for engineering plastics range from semiconductor Milling . . . . . . . . . . . . . . . . . . . . . . . . 19
processing equipment components to heavy equipment wear parts, to food Turning . . . . . . . . . . . . . . . . . . . . . . . 21
processing industry components.
Machinable plastic stock shapes (sheet, rod, and tube) are now available in
more than 50 grades, spanning the performance/price range of both ferrous
and non-ferrous metals to specialty ceramics. Plastics capable of long term
service up to 300°C, with short term exposures to 500°C are now available. As
the number of material options has increased, so has the difficulty of selecting
the right material for a specific application.
2 You inspire … we materialize®
The following guidelines are presented for those thumb for machining tolerances on plastics is 0.1 to 0.2% of the nominal size
machinists not familiar with the machining although tighter tolerances are possible with very stable, reinforced materials.
characteristics of plastics. They are intended as
guidelines only, and may not represent the most Quadrant Engineering Plastic Products’ stock shapes can be easily machined on
optimum conditions for all parts. The trouble- ordinary metalworking and in some cases on woodworking machines. However,
shooting quick reference guides in this booklet there are some points which are worth noting to obtain improved results.
should be used to correct undesirable surface
In view of the poor thermal conductivity, relatively low softening and melting
finishes or material responses during machining
temperatures of thermoplastics, generated heat must be kept to a minimum
operations. All Quadrant materials are stress
and heat build up in the plastics part avoided. This is in order to prevent
relieved to ensure the highest degree of machi-
deformations, stresses, colour changes or even melting.
nability and dimensional stability. Compared to
metals, however, the higher coefficient of thermal Therefore:
expansion, lower stiffness and higher elasticity • Tools must be kept sharp and smooth at all times (ground cutting edges),
as well as eventual swelling due to moisture • Feed rates should be as high as possible,
absorption (mainly with nylons) and possible • Tools must have sufficient clearance so that the cutting edge only comes in
deformations caused by internal stress-relieving contact with the plastic material,
during and after machining, generally result in • A good swarf removal from the tool must be assured,
greater difficulty maintaining tight tolerances • Coolants should be applied for operations where plenty of heat is generated
during and after machining. A good rule of (e.g. drilling).
When machining Quadrant stock shapes, remember...
• Thermal expansion is up to 20 times greater with plastics than with metals.
• Plastics lose heat more slowly than metals, so avoid localized overheating.
• As engineering plastics are not as rigid
• Softening (and melting) temperatures of plastics are much lower than those of as metals, it is essential to support
metals. the work adequately during machining
• Plastics are much more elastic than metals. in order to prevent deflection or
• High speed steel tools work well with
Because of these differences, you may wish to experiment with fixtures, tool many plastics.
materials, angles, speeds and feed rates to obtain optimum results.
• For long runs, use tungsten carbide,
ceramic or polycrystalline diamond
• Polycrystalline diamond tooling pro-
vides optimum surface finish when
machining celazole pbi or torlon pai.
4 You inspire … we materialize®
• Exept for drilling and parting, coolants are not typically necessary for thermoplastic machining operations.
• Keeping the cutting area cool generally improves surface finish and tolerances.
• When coolants are required, water-soluble coolants generally do very well. They should, however, not be used when machi-
ning amorphous thermoplastics, such as PC 1000, RADEL® PPSU 1000, ULTEM® PEI 1000, PSU 1000 and SEMITRON®
ESd 410C, because these materials are susceptible to environmental stress-cracking. The most suitable coolants for these
materials are pure water or compressed air.
• When the use of water-soluble coolants or general purpose petroleum based cutting fluids cannot be avoided during the
machining of amorphous thermoplastics (e.g. during drilling of large diameters and/or deep holes or during tapping operations),
the parts should immediately after machining be thoroughly cleaned with isopropyl alcohol first and rinsed with pure water
afterwards in order to reduce the risk of stress-cracking.
Quadrant Engineering Plastic Products’ stock shapes are annealed using a proprietary stress-relieving cycle to minimise any
internal stresses that may result from the manufacturing process.
This annealing procedure generally assures optimum dimensional stability during and after machining. However, when machining
parts that have to meet stringent requirements with respect to dimensional stability (tolerances, distortion, warpage,...) and/or
when machining causes asymmetric and/or heavy section changes, it is recommended to apply an intermediate annealing
procedure after pre-machining and prior to final machining of the part.
Annealing can be done in an air or preferably a nitrogen circulating oven, or in an oil bath.
6 You inspire … we materialize®
T1: heat-up time (heating rate: 10 – 20°C/hour)
T2: hold-time (depends on the wall thickness:
10 minutes per mm part thickness)
T3: cool-down time (cooling rate: 5 – 10°C/hour)
T4: additional time required to establish normal
(1) Temperature in the centre of the plastic part room temperature (depends on the wall
thickness: 3 minutes per mm part thickness)
(2) Oven or oil temperature
TIPS FOR ANNEALING
• When pre-machining, leave enough oversize to
allow machining to final sizes after annealing.
• Fixturing parts to desired shape or flatness
during the entire annealing cycle often proves
• Do not unfixture until parts have completed entire
Time annealing cycle and are cool to the touch.
RT • Make sure that temperatures are uniform and within
T1 T2 T3 T4 +/- 3°C all over the oven or the oil bath at all times
during the annealing cycle.
RT : room temperature - TH : hold-temperature • Do not take short-cuts.
Materials Heat up Hold temperature Hold-time (T2) Cool Down Environment(*)
PA 10-20 °C/h 150°C 10 min/mm 5-10°C/h air, nitrogen or oil
POM 10-20 °C/h 150°C 10 min/mm 5-10°C/h air, nitrogen or oil
PET 10-20 °C/h 150°C 10 min/mm 5-10°C/h air, nitrogen or oil
PE-(U)HMW 10-20 °C/h 80°C 10 min/mm 5-10°C/h air, nitrogen or oil
PC 10-20 °C/h 130°C 10 min/mm 5-10°C/h air or nitrogen
PEEK 10-20 °C/h 250°C 10 min/mm 5-10°C/h air, nitrogen or oil
PPS 10-20 °C/h 200°C 10 min/mm 5-10°C/h air, nitrogen or oil
PPSU 10-20 °C/h 200°C 10 min/mm 5-10°C/h air or nitrogen
PEI 10-20 °C/h 200°C 10 min/mm 5-10°C/h air or nitrogen
PSU 10-20 °C/h 170°C 10 min/mm 5-10°C/h air or nitrogen
PVDF 10-20 °C/h 140°C 10 min/mm 5-10°C/h air, nitrogen or oil
(*): when annealing in air, a more or less pronounced colour change of the outer surface is to be expected (particularly with nylons) – the thin oxidised surface-layer involved, however,
is most of the time removed during further machining operations.
8 You inspire … we materialize®
Plastics can build up heat very easily during drilling operations, especially when hole depths are greater than twice the diameter.
Therefore a cooling liquid is generally recommended.
• Small diameter holes (0.5 - 25 mm diameter)
High speed steel twist drills generally work well. In order to improve heat and swarf removal, frequent pull-outs (peck-drilling)
are necessary. A slow spiral (low helix) drill will allow for better swarf removal.
• Large diameter holes (25 mm diameter and larger)
It is advised to use drills with a thinned web (dubbed drill) in order to reduce friction and hence heat generation.
Drill large holes stepwise: a bore diameter of 50 mm e.g. should be made by drilling successively with Ø 12 mm and
Ø 25 mm, then by expanding the hole further with large diameter drills or with a single point boring tool.
10 You inspire … we materialize®
For the following materials it is recommended to bore holes in round rods
on a lathe, using “insert drills” or a rigid, flat boring tool with its cutting edge
perfectly set on centre-height (see drawing on the right).
• Rods > 50 mm diameter:
CELAZOLE® PBI, TORLON® PAI, KETRON® PEEK-HPV, KETRON®
PEEK-GF30, KETRON® PEEK CA30, TECHTRON® HPV PPS and
SEMITRON® ESD 410C.
• Rods > 100 mm diameter:
ERTALON® 66-GF30, ERTALYTE®, ERTALYTE® TX and
• Rods > 200 mm diameter:
ERTALON® and NYLATRON®.
Note: for these materials, some machinists prefer to heat the stock shapes up
to about 120 - 150°C prior to drilling.
α: relief angle (°)
A γ : rake angle (°)
φ: top angle (°)
� v : cutting speed (m/min)
s : feed (mm/rev.)
12 You inspire … we materialize®
Drilling - Troubleshooting
Difficulty Feed Marks or
Tapered Burned or Melted Chipping of
Difficulty Chatter Spiral Lines on
Hole Surface Surfaces
Common 1. Incorrectly 1. Wrong type drill 1. Feed too heavy 1. Too much 1. Feed too heavy
Cause sharpened oil clearance
2. Incorrectly 2. Clearance too 2. Drill not
2. Insufficient sharpened oil great 2. Feed too light centered
clearance 3. Feed too light 3. Too much rake 3. Drill overhang 3. Drill ground
3. Feed too heavy 4. Web too thick (thin web as too great off-center
described) 4. Too much rake
(thin web as
14 You inspire … we materialize®
Oversize Undersize Holes Not Rapid Dulling
Burr at Cut-off
Holes Holes Concentric of Drill
1. Drill ground 1. Dull drill 1. Feed too heavy 1. Dull cut-off tool 1. Feed too light
off-center 2. Too much 2. Spindle speed too slow 2. Drill does not 2. Spindle speed
2. Web too thick clearance 3. Drill enters next piece too far pass comple- too fast
3. Insufficient 3. Point angle too tely through 3. Insufficient
4. Cut-off tool leaves nib, which piece
clearance small deflects drill lubrication from
4. Feed rate too coolant
5. Web too thick
6. Drill speed too heavy at start
5. Point angle too
great 7. Drill not mounted on center
8. Drill not sharpened correctly
Proper clamping of shapes on worktable is required to avoid vibrations and
consequent rough cutting or even rupture. SAWING TIPS
• Tungsten carbide tipped saw blades
wear well and provide optimum surface
Band saws, circular saws or reciprocating saws need to have widely spaced
finishes ; particularly alternate top bevel
teeth, to assure good chip removal. They should have enough set to minimize
and triple chip grinds yield smooth cuts
the friction between the saw and the work and also to avoid close-in behind
with little or no chipping or burrs.
the cutting edge, causing excessive heat build-up and even blocking of the
Reinforced materials such as ERTALON® 66-GF30, TORLON® 4301 PAI,
TORLON® 4501 PAI, TORLON® 5503 PAI, KETRON® PEEK-HPV, KETRON®
PEEK-GF30, KETRON® PEEK-CA30, TECHTRON® HPV PPS, SEMITRON®
ESd 410C and SEMITRON® ESd 520HR are preferably cut with a brand saw
which has a tooth pitch of 4 to 6 mm (CELAZOLE® PBI: 2-3 mm). Do not use
circular saws, as this usually leads to cracks.
16 You inspire … we materialize®
Circular saw Circular saw Band saw Band saw
(carbide tipped) (carbide tipped)
tc tc tb tb
�c �c �b �b
�c X �c X
� c � circular saw
b : band saw
� = 10 – 15 α relief
� = 10 –: 15 angle (°)
γ : rake angle (°)
t : pitch (mm)
v : cutting speed (m/min)
Two flute end mills, face mills and shell mills with inserts as well as fly cutters
can be used for milling thermoplastics.
• Thin workpieces are often fixed
Climb milling is recommended to help reduce heat by dissipating it into the
onto the work table by means of
chip, and melting and poor surface finishes are minimized.
suction plates or double-sided
α: relief angle (°)
γ : rake angle (°)
v : cutting speed (m/min)
s : feed (mm/tooth) γ
Climb Milling vs. Conventional Milling
CUTTER CUTTER CUTTER CUTTER
ROTATION ROTATIONROTATION ROTATION
TABLE FEED TABLE FEED
TABLE FEED TABLE FEED
CLIMB MILLING CLIMB MILLING
CONVENTIONAL MILLING CONVENTIONAL MILLING
20 You inspire … we materialize®
Typical turning tool with tungsten carbide insert TURNING TIP
• The continuous chip stream pro-
5° duced when turning and boring many
thermoplastics can be handled well
5° using a compressed air powered suc-
tion system (directly disposing the swarf
Insert onto a container), in this way avoiding
the chip wrapping around the chuck,
the tool or the workpiece.
Turning & Boring Troubleshooting
Difficulty Cracking or
Melted Rough Burrs at Edge
Difficulty Chipping of Chatter
Surface Finish of Cut
Common 1. Tool dull or 1. Feed too 1. No chamfer 1. Too much positive 1. Too much
Cause heel rubbing heavy provided at sharp rake on tool nose radius on
2. Insufficient 2. Incorrect corners 2. Tool not eased tool
side clearance clearance 2. Dull tool into cut (tool sud- 2. Tool not
3. Feed rate too angles 3. Insufficient side denly hits work) mounted
slow 3. Sharp point clearance 3. Dull tool solidly
4. Spindle speed on tool (slight 4. Lead angle not 4. Tool mounted 3. Material not
too fast nose radius provided on tool below center supported
required) (tool should ease properly
4. Tool not out of cut gradu- 4. Depth of cut
mounted on ally, not suddenly) too heavy
center (use 2 cuts)
22 You inspire … we materialize®
Parting (Cutting-off) - Troubleshooting
Difficulty Concave or Nibs orBurrs Burns on
Melted Rough Spiral
Difficulty Convex at Cut-off Outside
Surface Finish Marks
Surfaces Point Diameter
Common 1. Dull tool 1. Feed too 1. Tool rubs 1. Point angle not 1. Point angle 1. No chamfer
Cause heavy during its great enough not applied before
side 2. Tool retreat 2. Tool not great enough cut-off
clearance improperly 2. Burr on perpendicular 2. Dull tool 2. Dull tool
3. Insufficient sharpened point of to spindle 3. Feed too
coolant tool 3. Tool deflecting heavy
supply 4. Feed too heavy
5. Tool mounted
above or below
r = 0.5 – 1 mm
B α: side relief angle (°)
γ : rake angle (°)
η: side cutting edge angle (°)
v : cutting speed (m/min)
s : feed (mm/rev.)
24 You inspire … we materialize®